Bio-DEE Synthesis and Dehydrogenation Coupling of Bio-Ethanol to Bio-Butanol over Multicomponent Mixed Metal Oxide Catalysts

Within the Waste2Fuel project, innovative, high-performance, and cost-effective fuel production methods from municipal solid wastes (MSWs) are sought for application as energy carriers or direct drop-in fuels/chemicals in the near-future low-carbon power generation systems and internal combustion engines. Among the studied energy vectors, C1-C2 alcohols and ethers are mainly addressed. This study presents a potential bio-derived ethanol oxidative coupling in the gas phase in multicomponent systems derived from hydrotalcite-containing precursors. The reaction of alcohol coupling to ethers has great importance due to their uses in different fields. The samples have been synthesized by the co-precipitation method via layered double hydroxide (LDH) material synthesis, with a controlled pH, where the M(II)/M(III) ≈ 0.35. The chemical composition and topology of the sample surface play essential roles in catalyst activity and product distribution. The multiple redox couples Ni2+/Ni3+, Cr2+/Cr3+, Mn2+/Mn3+, and the oxygen-vacant sites were considered as the main active sites. The introduction of Cr (Cr3+/Cr4+) and Mn (Mn3+/Mn4+) into the crystal lattice could enhance the number of oxygen vacancies and affect the acid/base properties of derived mixed oxides, which are considered as crucial parameters for process selectivity towards bio-DEE and bio-butanol, preventing long CH chain formation and coke deposition at the same time.


Introduction
Thirty years ago, in 1990, the first report of the Intergovernmental Panel on Climate Change (IPCC) was released, aiming to (1) summarize existing scientific knowledge on anthropogenic climate change, (2) assess the impact of climate change on humanity, and (3) identify solutions to the problem [1]. The world's energy resources and consumption have been determined in terms of greenhouse gas (GHG) emissions by applying predictive models. Currently, it is expected that advanced biofuels and alternative fuels will play an increasingly pivotal role in the gradual substitution of fossil fuels with fuels of renewable Acid-base properties in Mg-Al mixed oxides, generally known to be crucial for catalytic activity and selectivity, strongly depend on their chemical compositions and preparation procedures [48,52]. Although much is now known about the properties of hydrotalcite-based materials, the composition and structure of the active sites and reaction mechanism of ethanol coupling to butanol have not been clearly defined.
In this work, the development of heterogeneous catalysts for the conversion of ethanol into commodity chemicals is discussed. Ni-based catalysts obtained from hydrotalcitecontaining precursors were synthesized and studied. The effect of different divalent and triand four-valent cations (Ca 2+ , Mg 2+ , Ni 2+ /Ni 3+ , Cr 2+ /Cr 3+ /Cr 4+ , Mn 2+ /Mn 3+ /Mn 4+ , Al 3+ , Zr 4+ ) presence in the HTs precursor-containing framework on the performance of the mixed oxide catalysts was investigated. This work aims to elucidate the site requirements for ethanol coupling to butanol and diethyl ether (DEE) over the hydrotalcite-based materials and the mechanism by which this process occurs.

Catalyst Characterization
The chemical compositions of the mixed oxide active phases are shown in Table 1. These data confirm that the obtained compositions of all WP samples are close to the intended ones based on the ratios of the key elements of the Al component.  Figure 1 shows the XRD patterns of active phase precursors obtained by the standard co-precipitation method ( Figure 1A) as well as calcined and spent catalyst samples ( Figure 1B,C, respectively).
Pristine (only dried) WP1 hydrotalcite-like materials showed broad reflections attributable to a crystalline hydrotalcite phase, with indexing following the previously reported data (reflections at 2θ equal to 11 • , 23 • , and 35 • ; JCPDS 22-0452) [53,54]. These data suggest the isomorphic substitution of Mg 2+ by Ni 2+ in hydrotalcite brucite-like layers, which is in agreement with similarity in the effective ionic radius of those two components (Table 2) [55,56]. However, it is worth noting that the peaks related to the hydrotalcite phase are broad, and their intensity decreased with increasing content of the different divalent and tri-and four-valent cations (Ca 2+ , Mg 2+ , Ni 2+ /Ni 3+ , Cr 2+ /Cr 3+ /Cr 4+ , Mn 2+ /Mn 3+ /Mn 4+ , Al 3+ , Zr 4+ ). This can indicate indicating a more disordered structure, changes in layer-spacing or a decrease in crystallinity [55][56][57][58]. Additionally, for Mgcontaining samples, traces of crystalline Al(OH) 3   Pristine (only dried) WP1 hydrotalcite-like materials showed broad reflections attributable to a crystalline hydrotalcite phase, with indexing following the previously reported data (reflections at 2θ equal to 11°, 23°, and 35°; JCPDS 22-0452) [53,54]. These data  The formation of bimetallic solids between Ni and Al can be explained by the insertion of Al 3+ ions (69 pm) in the NiO crystal lattice, which, due to the lower ionic radius of Al 3+ , leads to the decrease in the dimensions of NiO cubic cells. This insertion is allowed as the size of the Al 3+ does not differ by more than 15% from that of the Ni 2+ (72 pm), and it crystallizes in the cubic system in the form of transition alumina that can be formed by calcination. Moreover, it has an electronegativity close to that of nickel, which complies with three of the Hume-Rothery rules. For Ca-containing samples, the presence of CaCO 3 (vaterite modification) was observed, consistent with the previously reported data for calcium carbonate samples [57,58]. Additionally, intensity decrease and broadening of XRD pattern reflexes were observed ( Figure 1A), suggesting incompatibility between the charge (Cr 4+ , Mn 4+ , Zr 4+ ) and the ionic radius of selected elements (Table 2) of the dopant and the crystal structure of the brucite layer in HT-like material [51]. The HT-like phase structure collapsed for samples calcined at 823 K, and different phases were detected in the XRD diffraction patterns ( Figure 1B). The reflections characteristic of the periclase-like structure of mixed oxides (reflections at 2θ equal to 37 • , 43.5 • , 63 • ) were the most intense [55]. Some overlapping signals related to NiO (JCPDS 65-5745) and Al 2 O 3 (JCPDS 04-0880) were also observed. In the samples containing calcium, CaCO 3 phase transformation to calcite was evidenced with sharp reflections located at 2θ equal to 37 • , 43.5 • , 63 • . This result shows that the calcination performed at 823 K was sufficient to transform the hydrotalcite and bayerite phases into the corresponding oxide forms but was too low to cause the CaCO 3 decomposition. All detected phases in calcined samples were present in samples after reaction ( Figure 1C), suggesting good structure stability of the samples. The BET area (A BET ) measured for the calcined samples stayed roughly constant at around 210 m 2 /g in both types of samples (Mg-containing WP-1, WP-2, and WP-3) or Ca-containing ones (WP-4, WP-5). Figure 2 shows SEM and TEM images of the calcined (WP-1-WP-5) and after reaction (WP-1AR-WP-5AR) samples. All catalysts obtained from hydrotalcite-like precursors were composed of plate-like particles (Figure 2, WP-1-WP-5). The sample morphology was not changed, comparing both Mg-containing or Ca-containing samples to the pristine WP-1 sample. Moreover, this morphology has been preserved in all samples after reaction ( Figure 2, WP-1AR-WP-5AR). TEM images of calcined samples (WP-1 -WP-5'), shown in Figure 2, reveal some differences in the microstructures of prepared catalysts. In all samples, the active mixed oxide phase particles are visible as black and/or dark grey grains, dispersed among the amorphous phase. In all Cr-, Mn-, and Zr-doped catalysts obtained from HT-like precursors, the calcined, mostly Ni-metal-based active phase forms oxide particles stayed in the range 5-6 nm. Catalysts 2021, 11,660 The DRIFT spectra of calcined samples are shown in Figure 3. The DRIFT spectra of calcined samples are shown in Figure 3.   The spectrum recorded for WP-1 shows three broad complex absorptions with maxima located at 700-1200, 1250-1750, and ca. 3500 cm −1 , in accordance with previous studies [33,55,59,60]. The broad band at 3470 cm −1 was ascribed to the OH stretching mode ν(OH)of structural hydroxyl groups. The corresponding H-O-H bending mode of physisorbed water was evidenced at 1632 cm −1 . The band at 1763 cm −1 corresponds to the presence of some interlayer water. The appearance of this vibration in the spectra is most likely explained by the "memory effect" of the calcined powder sample or incomplete decomposition of the layered structure during calcination [55,59,60]. The bands in the 700-1200 and 1250-1750 cm −1 spectral regions are characteristic of carbonate vibrations. For all HT-derived samples (WP-1-WP-5), the recorded spectra were similar and presented the most intense band, located at 1034 cm −1 . According to the previous research, this peak can be ascribed to the ν1 mode of carbonate [61]. Usually, this mode stays IR-inactive due to the symmetry rules. However, in the interlayer, the D 3h symmetry of free carbonate is lowered to C 3v or C 2v , and it becomes activated. For WP-4 and WP-5 samples, displacement and splitting of this band were observed, which can be related to the calcite presence, where the local symmetry of carbonate was D 3 [61]. These results are in good agreement with the XRD measurement, where the presence of calcite has been evidenced for Ca-containing samples (WP-4 and -5). The bands recorded below 1000 cm −1 can be due to the carbonate (ca. 850 cm −1 ) and M-OH modes. Moreover, these features are also typical of the spinel structure and can be related mainly to the formation of γ-Al 2 O 3 and (Mg/Mn/Cr/Zr)Al 2 O 4 , as the bands at low wavenumbers (usually at 700 and 570 cm −1 ) are assigned to the so-called ν 1 and ν 2 vibrational mode of isolated tetrahedra, i.e., [AlO 4 ] and octahedra, i.e., [AlO 6 ], respectively [55,60].
The Raman spectra of the calcined WP-1-WP-5 samples before and after the reaction are presented in Figure 4. A broad signal around 551 cm −1 was also observed for all the materials. This signal was related to octahedral Ni 2+ species. Usually, the Raman spectra of nickel oxide are reported to possess five bands that originate from the optical vibrations produced by one phonon (1P) of the transverse optical (TO-440 cm −1 ) and longitudinal optical (LO-560 cm −1 ) and by two phonons (2P). As a result of the TO+TO TO+LO and LO+LO coupling, three scatterings were further observed at 730, 930, and 1080 cm −1 [62][63][64]. The Raman spectra of all the calcined WP samples mainly displayed the band originating from the 1P scattering at 551 cm −1 , whereas bands related to the 2P coupling were not identified. This band is considered as characteristic of nickel oxide with alterations in its crystalline structure, which may be due to vacancies created by the non-stoichiometric Ni 1-x O oxide or the Ni 3+ presence in the structure [64]. The presence of smaller Al 3+ ions in the NiO lattice may cause the formation of crystalline defects and vacancies, favoring the 1P interaction. It is noteworthy that, when traces of Mn, Cr, and Zr are present in the structure, the band at 551 cm −1 is wider, and blue shifted. This can be explained by the formation of more defects and vacancies by dopant ions and/or by the band coincidence with the lattice vibration of the hydroxyl layers of these metals [62][63][64]. In Figure 4B, the Raman spectra of the WP-X samples after the reaction are shown. It was noticed that signals associated with the carbon are intense, shielding the metal signals. The Raman spectra showed two characteristic peaks at 1585 and 1350 cm −1 related to the G and D bands. The G band corresponds to the stretching vibration between the C-C bonds along the longitudinal axis of the graphite plane. In contrast, the D band refers to association with the presence of amorphous carbon, disordered crystal structure, or crystal defects [65,66]. The bands were deconvoluted as described previously; however, other bands (D 2 , D 3 , D 4 ) were not detected [67]. The graphitic index (I G ) of the samples was calculated from the deconvolution of the signals, and the value for all the materials was around 25%. The collected spectra revealed that the carbon formation during the carried reaction was the highest for the WP-1 sample. In general, the Mg-containing catalysts contained more coke after the coupling reaction, and they were more active than Ca-containing catalysts ( Table 3).      Figure 5 presents the effect of metal type content on the catalytic performance during EtOH coupling reactions. At the investigated reaction conditions (350 • C, ambient pressure; GHSV= 1.19 × 10 5 h −1 ), the MgAl catalyst had a very low alcohol conversion (EtOH conv. ∼10%) but high C-selectivity to n-butanol and ethyl ether (>40%). Ethanol coupling occurred in the same temperature range for all the catalysts. There are several differences in terms of activity, defined as conversion after 100 min and selectivity towards DEE and n-butanol ( Table 3). Incorporation of Ni in MgAlO (WP-2) afforded a selectivity of 46% to nbutanol with an ethanol conversion of 15%. However, the NiAlCO 3 sample (WP-1) showed high ethanol conversion (97%), but the selectivity of n-butanol and ethyl ether decreased. Indeed, for the NiAlCO 3 sample, apart from the product decomposition, the products' distribution changed, suggesting C-C coupling omittance, as was given previously [11]. This is due to the well-known ability of Ni in the form of NiO to activate C-H and O-H bonds in alcohols to form the corresponding aldehydes and also due to the more acidic nature of the surface composition determining the reaction pathway [11].  For the WP-3 catalyst (Mn, Cr, and Zr-modified Ni-Mg-Al mixed oxide), the highest activity was observed in terms of ethanol conversion with selectivity toward DEE approaching 60% ( Figure 5). This behavior is most likely due to the introduction of Mn 4+ For the WP-3 catalyst (Mn, Cr, and Zr-modified Ni-Mg-Al mixed oxide), the highest activity was observed in terms of ethanol conversion with selectivity toward DEE approaching 60% ( Figure 5). This behavior is most likely due to the introduction of Mn 4+ species in the Mg-based structure, and Mg 2+ species are more active for the aldol condensation reaction. Thus, n-butanol formation was inhibited [39]. Other studies have also reported that enhanced dehydration can be promoted instead. This is due to the interaction between Mg 2+ and Al 3+ that weakens the metal-support interaction as well as due to the decrease in Mg/Al ratio [40,41]. The data presented in Figure 5 demonstrate that the promotor of ethanol's coupling reaction is the Mg-Al hydrotalcite precursor, which is in agreement with the literature [24,26,32,39,61,68].

Catalytic Performance
Mechanistic studies of alcohol (methanol+n-propanol, ethanol) coupling reactions on mixed metal oxides (MgAlO x ) have revealed that an optimum population of weak Lewis acid and strong Brønsted base-pair sites resulting from intimate contact of Mg and Al oxide phases is required for maximizing the C-C coupling reaction rates that are not achieved with either monometallic oxides MgO (mostly basic), or Al 2 O 3 , (mostly acidic) [24,68,69]. DiCosimo et al. have shown that on MgAlO x mixed metal oxides (atomic Mg/Al = 1), the maximum ethanol coupling formation rate to n-butanol coincides with the maximum density of basic sites in the catalyst [68,69]. In the present work, we report vapor-phase coupling reactions of ethanol on mixed metal oxides at varying metal contents aimed at maximizing the C-C coupling product for ethanol.
In the vapor phase, the main reported reaction pathways for the C-C coupling of lower alcohols to higher alcohols on multimetallic mixed oxides include several reactions, as proposed by J.J. Bravo-Suárez et al. [24].
Aldol condensation of aldehydes with the elimination of water (C-C bond-forming) to an aldehyde: 3.
Additionally, allylic aldehyde reduction (hydrogenation) to alcohol: Other reactions that have been proposed include direct alcohol and aldehyde condensation (to C-C coupled intermediate species), hydroxy aldehyde keto-aldol interconversion, reverse aldol coupling (to keto form), esterification reactions from aldehydes and surface alkoxides, and ethanol decarbonylating (decomposition).
During the coupling reaction, the water was formed, but the water's presence does not harm the catalysts' structures and morphologies, evidenced by XRD (Figure 1c) and SEM ( Figure 2). All catalysts preserve a mixed oxide structure. The water could remove the coke by gasification; however, for these catalysts, this route apparently did not occur with a high conversion level at the temperatures used [42].
The direct transformation of ethanol into 1-butanol is described as being catalyzed by solid bases [70]. For such catalysts, mechanistic studies have shown that ethanol dimerization is the preferred mechanism, which is usually supported by the fact that expected reaction intermediates are detected [71,72]. In general, two alternative mechanisms have been proposed for alcohol coupling, namely, a Guerbet reaction or a direct condensation mechanism ( Figure 6) [71,72]. In the Guerbet reaction, the C-C formation occurs via aldol condensation. This reaction includes dehydrogenation of ethanol to an aldehyde (often identified as the rate-limiting step), followed by aldol-type condensation of aldehyde and transfer hydrogenation (TH) of polarized substrates [73,74]. Most likely, for studied WP-X catalysts, both H 2 and produced H 2 O can act as hydrogen donors, as suggested earlier [73]. In the second mechanism, i.e., direct condensation, the first activation of the β-H of ethanol molecule is followed by the condensation with another ethanol via dehydration [74]. Thus, dual functionality of catalytic systems is required to provide desirable Guerbet conversion and selectivity, where one component is active in ethanol dehydrogenation and support or/and the second component shapes the acetaldehyde aldolization selectivity. Until now, various transition metals have been reported to enhance ethanol dehydrogenation, aiming to improve ethanol conversion under mild conditions [72,74]. Incorporation of Ni to LDH-derived catalysts showed promising activity with high selectivities related to the acid-base site modification of WP-X catalysts' surfaces. In the Ag-supported MgAl-LDO catalyst, the basic sites promote the adsorption and subsequent dehydrogenation of ethanol on uniformly dispersed Ag particles [74]. Thus, the acid-base cooperation was ascribed to promote the C-C bond formation of dehydrogenated intermediate via aldol condensation. In the case of investigated WP-X, Ni most likely acts as a hydrogentransfer component. Simultaneously, the presence of the multiple redox couples Ni 2+ /Ni 3+ , Cr 2+ /Cr 3+ , Mn 2+ /Mn 3+ , and the oxygen-vacant sites affect the acid/base properties of derived mixed oxides. This dual functionality is of crucial importance for the process selectivity towards bio-DEE and bio-butanol. This complex issue is currently under detailed investigation by our group.

Structural Changes of Catalyst
The average Raman spectra of WP1 before and after the reaction are present in Figure  7A,B, respectively. The spectrum of the sample before the reaction displays bands at 391 cm −1 , originating from the A1 phonon mode of Al 3+ or Ni 2+ species, at 562 cm −1 , ascribed to phonon mode of Ni 2+ species, at 816 cm −1 , corresponding to the condensed tetrahedral AlO4, at 1104 cm −1 , assigned to νCO3 2− ion, and at 1605 cm −1 , from an unknown source [1][2][3][4].
The spectrum of the after-reaction sample contains bands at 383 cm −1 , corresponding to the A1 phonon mode of Al 3+ or Ni 2+ species, and at 522 cm −1 , ascribed to the phonon mode of Ni 2+ species. The band at 816 cm −1 , corresponding to condensed tetrahedral AlO4, Until now, various transition metals have been reported to enhance ethanol dehydrogenation, aiming to improve ethanol conversion under mild conditions [72,74]. Incorporation of Ni to LDH-derived catalysts showed promising activity with high selectivities related to the acid-base site modification of WP-X catalysts' surfaces. In the Ag-supported MgAl-LDO catalyst, the basic sites promote the adsorption and subsequent dehydrogenation of ethanol on uniformly dispersed Ag particles [74]. Thus, the acid-base cooperation was ascribed to promote the C-C bond formation of dehydrogenated intermediate via aldol condensation. In the case of investigated WP-X, Ni most likely acts as a hydrogentransfer component. Simultaneously, the presence of the multiple redox couples Ni 2+ /Ni 3+ , Cr 2+ /Cr 3+ , Mn 2+ /Mn 3+ , and the oxygen-vacant sites affect the acid/base properties of derived mixed oxides. This dual functionality is of crucial importance for the process selectivity towards bio-DEE and bio-butanol. This complex issue is currently under detailed investigation by our group.

Structural Changes of Catalyst
The average Raman spectra of WP1 before and after the reaction are present in Figure 7A,B, respectively. The spectrum of the sample before the reaction displays bands at 391 cm −1 , originating from the A 1 phonon mode of Al 3+ or Ni 2+ species, at 562 cm −1 , ascribed to phonon mode of Ni 2+ species, at 816 cm −1 , corresponding to the condensed tetrahedral AlO 4 , at 1104 cm −1 , assigned to νCO 3 2− ion, and at 1605 cm −1 , from an unknown source [1][2][3][4].
bands were located in the specific sample areas. They were not correlated with the catalyst band occurrence, which proves that the reaction was complete and the catalyst did not degrade during the catalytic reaction (which was also proven when taking into account the averaged spectra). Moreover, D and G bands were distributed in the same sample locations, proving that the production of imperfect and perfect graphite or graphene needs the same conditions. The average Raman spectra of WP2 before and after the reaction are present in Figures 8A,B, respectively.
The WP2 spectrum displays bands at 391 cm −1 , originating from the A1 phonon mode of Al 3+ or Ni 2+ species, at 562 cm −1 , ascribed to the phonon mode of Ni 2+ species, at 1084 cm -1 , corresponding to either the two phonon modes of Ni 2+ species or νCO3 2− ion, at 1168 The spectrum of the after-reaction sample contains bands at 383 cm −1 , corresponding to the A 1 phonon mode of Al 3+ or Ni 2+ species, and at 522 cm −1 , ascribed to the phonon mode of Ni 2+ species. The band at 816 cm −1 , corresponding to condensed tetrahedral AlO 4 , was present in the sample's spectrum before but not after the reaction. Moreover, the band at 1085 cm −1 appeared in the after-reaction sample. This band is ascribed to either two phonon modes of Ni 2+ species or νCO 3 2− ion [3]. The latter is more probable as a similar band was present in the sample's spectrum before reaction (at 1104 cm −1 ). Two additional bands, located at 1351 and 1578 cm −1 , are present in the sample's spectrum after the reaction. They are assigned to imperfect graphite (D band) and perfect graphite or graphene (G band), respectively [5]. Bands at~385 and~540 cm −1 are present in both samples' spectra. However, both bands are significantly shifted toward lower Raman shift values in the after-reaction sample's spectrum compared to that of the before-reaction sample. This result suggests a change in the catalyst structure. The band at~385 cm −1 has a comparable area under the curve in both samples. However, in the after-reaction sample's spectrum, the band at~540 cm −1 has a three-fold higher area compared to that before the reaction. This result might indicate the condensed tetrahedral AlO 4 (the band that disappeared in the after-reaction sample) transformation to octahedral AlO 6 , which might be found in the lower Raman Shift values [1]. The G and D bands were present in the after-reaction sample's spectrum, suggesting that the reaction product was a coke.
In the chemical maps of the before-reaction sample, all bands, except for the one at 1605 cm −1 , were evenly distributed throughout the sample. The band at 1605 cm −1 was observed on the sample surface, whereas the band at 816 cm −1 was absent. This result might indicate an incomplete reaction while creating the catalyst or uneven reaction throughout the sample. In the after-reaction sample's chemical maps, the bands corresponding to the catalyst were evenly distributed throughout the sample. The D and G bands were located in the specific sample areas. They were not correlated with the catalyst band occurrence, which proves that the reaction was complete and the catalyst did not degrade during the catalytic reaction (which was also proven when taking into account the averaged spectra). Moreover, D and G bands were distributed in the same sample locations, proving that the production of imperfect and perfect graphite or graphene needs the same conditions.
The average Raman spectra of WP2 before and after the reaction are present in Figure 8A,B, respectively. The average Raman spectra of WP4 before and after the reaction are present in Figure  9A,B, respectively.
In the after-reaction sample, the spectrum contains bands at 394 cm −1 , corresponding to the A 1 phonon mode of Al 3+ or Ni 2+ species, at 523 cm −1 , ascribed to the phonon mode of Ni 2+ species, at 1085 cm −1 , assigned to either the two phonon modes of Ni 2+ species or νCO 3 2− ion, at 1384 cm −1 , ascribed to the imperfect graphite (D band), and at 1578 cm −1 correspond to perfect graphite or graphene (G band) [5]. In the after-reaction sample, the band corresponding to the phonon mode of Ni 2+ species was significantly shifted toward a lower Raman shift value. It is probably due to the slight change in the catalyst structure. The band at 1168 cm −1 was not detected in the after-reaction sample; however, it might be overlapped by D and G bands. Moreover, in the after-reaction sample's spectrum, D and G bands were present. Although the G band was also present in the before-reaction sample's spectrum, the G band area in the after-reaction sample's spectrum was almost 7.5 times higher than that in the sample's spectrum before the reaction (1899 vs. 254), as visible in Figure 8A,B. This result shows that the sample induced coke production with very high abundance (higher than WP1).
Before the reaction, the chemical maps of the sample show that all catalyst bands were evenly distributed throughout the sample, proving the catalyst's chemical homogeneity. In the after-reaction sample, the chemical maps indicate that the intensity of the highest catalyst band (at 523 cm −1 ) was reversely proportional to the D and G bands. This result might suggest that the reaction was not complete and that the catalyst degraded as the reaction progressed. However, the latter is not true. The area of the band at 523 cm −1 in the after-reaction sample's spectrum was higher compared to that in the beforereaction sample's spectrum. The arguments mentioned above prove that the WP2 catalyst induced the coke production reaction with very high abundance and was stable in the used reaction conditions.
The average Raman spectra of WP4 before and after the reaction are present in Figure 9A,B, respectively.
The average spectrum of the sample before the reaction contains bands at 395 cm −1 , corresponding to the A 1 phonon mode of Al 3+ or Ni 2+ species, at 561 cm −1 , ascribed to the phonon mode of Ni 2+ species, at 804 cm −1 , corresponding to the condensed tetrahedral AlO 4 , at 1084 cm −1 , ascribed to either two phonon modes of Ni 2+ species or νCO 3 2− ion, and at 1142 cm −1 , from an unknown source [1][2][3][4].
The average spectrum of the after-reaction sample contains bands at 402 cm −1 , corresponding to the A 1 phonon mode of Al 3+ or Ni 2+ species, at 531 cm −1 , ascribed to the phonon mode of Ni 2+ species, at 787 cm −1 , corresponding to the condensed tetrahedral AlO 4 , at1084 cm −1 , ascribed to either the two phonon modes of Ni 2+ species or νCO 3 2− ion, and at 1345, 1579, and 1606 cm −1 , corresponding to the imperfect graphite (D band), perfect graphite or graphene (G band), and imperfect graphite or disordered carbon (D' band), respectively [5]. In the after-reaction sample's spectrum, the band at 531 cm −1 was significantly shifted towards lower Raman Shift values compared to that in the before-reaction sample's spectrum. This result could indicate slight changes in the catalyst structure. The band at 1142 cm −1 , present in the before-reaction sample, was not present in the afterreaction sample, probably due to the degradation or structural change in the substance corresponding to that band. Moreover, in the after-reaction sample, the D, G, and D' bands' presence proves that this catalyst induced coke production but with very low efficiency (based on the bands' area analysis). the main band of the catalyst, and the band at 1084 cm were distributed in specific sample regions, proving that the sample was not homogenous. In the after-reaction sample's chemical maps, all bands of the catalyst and its products were evenly distributed, except for the band at 1085 cm −1 . This band's intensity was the highest in a specific sample spot. Moreover, the intensity of all other bands was low in the same spot (except for the band at 787 cm −1 ). These results indicate that the sample was not homogenous, and the spot with high intensity of 1085 cm −1 band had low catalytic efficiency.

Synthesis and Characterization
The Ni-containing hydrotalcite-like precursors were synthesized by a co-precipitation method from an aqueous solution of appropriate nitrate salts. During the synthesis, the samples were prepared and denoted as WP1-WP5, respectively, with full composition given in Table 1. An identical synthetic procedure was applied in all cases, e.g., the WP1 The before-reactions sample's chemical maps consist of bands at 395, 804, and 1142 cm −1 that were evenly distributed throughout the sample. However, the band at 561 cm −1 , the main band of the catalyst, and the band at 1084 cm −1 were distributed in specific sample regions, proving that the sample was not homogenous. In the after-reaction sample's chemical maps, all bands of the catalyst and its products were evenly distributed, except for the band at 1085 cm −1 . This band's intensity was the highest in a specific sample spot. Moreover, the intensity of all other bands was low in the same spot (except for the band at 787 cm −1 ). These results indicate that the sample was not homogenous, and the spot with high intensity of 1085 cm −1 band had low catalytic efficiency.

Synthesis and Characterization
The Ni-containing hydrotalcite-like precursors were synthesized by a co-precipitation method from an aqueous solution of appropriate nitrate salts. During the synthesis, the samples were prepared and denoted as WP1-WP5, respectively, with full composition given in Table 1. An identical synthetic procedure was applied in all cases, e.g., the WP1 sample was synthesized as follows: Ni(NO 3 ) 2 ·6H 2 O, and Al(NO 3 ) 3 ·9H 2 O were dissolved in deionized water (135 mL) at a molar ratio of M 2+ /M 3+ of 0.35. The metallic salt solution was added dropwise into 370 mL of 0.2 M Na 2 CO 3 solution under vigorous stirring. During the synthesis process, the temperature was maintained at 328 K, and pH was kept at 10 by simultaneous addition of 1 M NaOH. The obtained products were collected by centrifugation, washed several times with distilled water, and dried at 323 K in air. Then, the dried solids were ground using an agate mortar. A similar procedure was used to obtain WP2-WP5 precursors. Finally, to prepare the mixed oxide materials, the hydrotalcite precursors were calcined in a muffle furnace at 823 K for 4 h.
The crystalline phases of all the synthesized hydrotalcite-like materials and the calcined products were determined from their XRD patterns, recorded using an X'Pert PRO PANalytical B.V. The X-ray diffractometer used Cu Kα radiation (40 kV, 30 mA) of 0.154 nm. The XRD data were collected between 2θ = 2 • and 72 • .
Raman spectra were collected in a Thermo Scientific DXR Raman Microscope, working at an exciter line of 532 nm and incorporating a Charge Couple Device (CCD) detector. Spectra were recorded in the 200-2000 cm −1 Raman shift range with an accumulation time of nearly 5 s, 10 mW of power, and 64 scans.
IR spectra of calcined samples were collected in a Nicolet iS50 FT-IR spectrometer. A built-in all reflective, mid-and far-IR diamond attenuated total reflectance (ATR) and diffuse reflectance (DRIFT) modules were used to record the IR spectra. Typically, 100 scans were collected at a resolution of 1 cm −1 and 2 mW of power.
SEM images were obtained using the field-emission scanning electron microscope (FE-SEM) FEI Nova NanoSEM 450 Series under vacuum ca. 10 −6 mbar. The WP catalyst sample powders were deposited onto the standard SEM specimen stub for precise positioning under the electron column for imaging. SEM images were collected using the Through Lens Detector (TLD) of secondary electrons at the primary beam energy of 10 keV and 4.8 mm working distance from the pole piece. All images were obtained at a long scan acquisition time (20 µσ) of typically 30 s per image after choosing the inspection region. HRTEM TITAN 60-300 instrument with an X-FEG-type emission gun operating at 80 kV was used to record TEM images. The microscope was equipped with a Cs image corrector and a STEM high-angle annular dark-field detector (HAADF); its point resolution is 0.06 nm in TEM mode.

Catalytic Tests
The ethanol coupling tests were performed in a tubular fixed-bed reactor (5 mm external diameter) equipped with an online mass spectrometer (MS). Typically, 40 mg of sieved catalyst (20-40 mesh) was loaded into the reactor, and the remaining was filled with quartz sand (20-40 mesh). Before the reaction, the catalyst was pre-treated in situ with He (50 mL min −1 ) at 773 K with a rate of 10 K s −1 for 3 h. Ethanol vapor and He were mixed into the reaction system after the reactor was cooled to 523 K. The gas flow was set to 60 mL min −1 . Before the ethanol admission into the reaction system, ethanol was vaporized at 423 K in a vaporizing chamber. The chromatographically pure ethanol was pumped into the vaporizing chamber at 50 µL min −1 using a high-performance liquid chromatography pump. The pipeline behind the reactor was heated to keep it at 473 K. The products were identified and analyzed by online MS (Hiden, HPR 60). The ethanol conversion and product selectivity were calculated as follows: X% = n in −n unreacted n in × 100% (4) S% = C mol of specific product C mol of products × 100% (5) C balance % = C mol of products C mol of conversed ethanol × 100% (6) S dehydrogenation % = 100% − S DEE % S C−C coupling % = ∑ S C 4 −C 4+ products % (8) where n in and n unreacted are the moles of initial and unreacted ethanol; C mol is the mole number of carbon in the products and conversed ethanol; S is the selectivity for DEE (M/z = 59, 74), and C 4 -C 4+ products, such as n-butanol

Raman Spectroscopy
The Raman spectra were collected using a confocal Thermo DXR Raman Microscope. The magnification of the objective was 50×, and the laser with 532 nm wavelength and 8 mW of power was used. The parameters were optimized before the analysis. The aperture was 50 µm pinhole, the exposure time was 4 s, and the number of exposures for one spectrum was 20. All the samples were measured in the range 250-2700 cm −1 ; however, only the 250-1750 cm −1 spectral region is shown. The whole map was 15 × 15 µm, and it was made with a step size of 1.5 µm/1.5 µm in the x/y axis direction. The spectra analysis (baseline correction, deconvolution) was performed using Origin Pro Software (v. 9.1, OriginLab Corporation, Northampton, MA, USA, 2013). The band frequencies, used for spectral deconvolution, were determined from the second derivative spectra. The chemical map analysis was carried out in CytoSpec (v. 2.00.01). Maps were normalized and baseline-corrected before the analysis.

Conclusions
The catalysts obtained from hydrotalcite-containing precursors have demonstrated a moderate activity in the dehydrogenation coupling of bio-ethanol to produce more caloric bio-fuels, namely, DEE and n-butanol. It was shown that, at given reaction conditions (623 K and 0.1 MPa), the highest conversion was obtained for the bare Ni 0.35 Al-CO 3 (WP-1) sample. Most likely, the basic sites highly influence catalyst activity. For the Ni and Mgcontaining catalyst (Ni 0.35 Mg 0.13 Al-CO 3, WP2), the ethanol dehydrogenation was carried out with the highest efficiency with the participation of Ni sites and aldol condensation promoted by acid-base cooperation. Further material modification with Cr, Zr, and Mn increased the redox and oxygen storage capacity (OSC), increasing the number of oxygen vacancies in the corresponding mixed oxide lattice. Thus, in the final WP-3 catalysts (Ni 0.35 Mg 0.13 Mn 0.0018 Cr 0.0017 Zr 0.0054 Al-CO 3 ), the aldol condensation was limited as the acidity increased, and the reaction seemed to be preferential towards DEE formation. Mg exchange on Ca during the catalyst precursor synthesis resulted in derived mixed oxides, with different basicities and/or different basic strength distributions, affecting the overall bio-ethanol conversion and selectivity towards DEE and n-butanol. The effect of promoters on the Ni particles' stability and the electronic effect on Ni in the dehydrogenation coupling of C 1 -C 2 bio-alcohols towards ethers and n-butanol is currently under detailed investigation under the Waste2Fuel project.
All studied catalysts demonstrated the ability to synthesize coke. The Ni 0.35 Mg 0.13 Al-CO 3, catalyst (WP2) demonstrated the highest efficiency, while the Ni-and Ca-containing catalyst (WP4) sample's efficiency was the lowest. All samples' structures changed during the reaction; however, WP1 and WP2 probably did not degrade under the reaction conditions used. The WP4 sample' structure was inhomogeneous.